received: 13 November 2015 accepted: 16 March 2016 Published: 11 April 2016
Helical Majorana fermions in d x 2 – y 2 + id xy -wave topological superconductivity of doped correlated quantum spin Hall insulators Shih-Jye Sun1, Chung-Hou Chung2,3, Yung-Yeh Chang2, Wei-Feng Tsai4 & Fu-Chun Zhang5,6 There has been growing interest in searching for exotic self-conjugate, charge-neutral low-energy fermionic quasi-particles, known as Majorana fermions (MFs) in solid state systems. Their signatures have been proposed and potentially observed at edges of topological superconcuctors with non-trivial topological invariant in the bulk electronic band structure. Much effort have been focused on realizing MFs in odd-parity superconductors made of strong spin-orbit coupled materials in proximity to conventional superconductors. In this paper, we propose a novel mechanism for realizing MFs in 2D spin-singlet topological superconducting state induced by doping a correlated quantum spin Hall (KaneMele) insulator. Via a renormalized mean-field approach, the system is found to exhibits time-reversal symmetry (TRS) breaking d x 2−y 2 + id xy -wave (chiral d–wave) superconductivity near half-filling in the limit of large on-site repulsion. Surprisingly, however, at large spin-orbit coupling, the system undergoes a topological phase transition and enter into a new topological phase protected by a pseudospin Chern number, which can be viewed as a persistent extension of the quantum spin Hall phase upon doping. From bulk-edge correspondence, this phase is featured by the presence of two pairs of counterpropagating helical Majorana modes per edge, instead of two chiral propagating edge modes in the d + id′ superconductors. Searching for topological states of quantum matters constitutes one of the central and fundamental issues in condensed matter systems. The growing interest in topological insulators (TIs), which support gapless edge (or surface) states protected by time-reversal symmetry (TRS) while the bulk remains insulating1,2, is one prime example. Of particular interest are topological superconductors which support gapless self-conjugate, charge-neutral fermionic quasi-particle excitations3. These excitations which reflect non-trivial topological bulk properties are localized at the edges, known as Majorana fermions (MFs). Much effort has been put in searching for signatures of Majorana fermions in solid state materials. One-dimensional semiconductor nano-wires with strong spin-orbit (SO) coupling under a magnetic field proximity to a s-wave superconductor have been proposed theoretically to host MF at both ends of the wire4–6, and also studied experimentally7–11. Similar ideas have been proposed in 2D systems where chiral MFs exist at the edges of spin-triplet, p–wave (odd-parity) superconductors12–14. While realization of the above systems relies on TRS breaking by the Zeeman field, time-reversal invariant topological superconductors (TRITOPs)15–18 have recently been proposed to host two time-reversal pairs of helical MFs at edges in repulsively interacting SO coupled nano-wire proximity to either a s-wave6,16 or a d–wave19 1
Department of Applied Physics, National University of Kaohsiung, Kaohsiung, Taiwan, R.O.C. 2Electrophysics Department, National Chiao-Tung University, HsinChu, Taiwan, 300, R.O.C. 3Physics Division, National Center for Theoretical Sciences, HsinChu, Taiwan, 300 R.O.C. 4Department of Physics, National Sun Yat-Sen University, Kaohsiung, Taiwan, R.O.C. 5Department of Physics, Zhejiang University, Hangzhou, China. 6Collaborative Innovation Center of Advanced Microstructures, Nanjing, China. Correspondence and requests for materials should be addressed to C.-H.C. (email: [email protected]
) Scientific Reports | 6:24102 | DOI: 10.1038/srep24102
Figure 1. Honeycomb lattice of a finite-sized zigzag ribbon of the tight-binding Kane-Mele t-J model with the ribbon size N = 8 being twice the number of zigzag chains along x-axis. Nearest-neighbor and nextnearest-neighbor lattice vectors are δa =1,2,3, ai = 1,2 with an unit length of a, a, respectively. We set a = 1 here. The gray shaded region represents for the super-unit-cell of the zigzag ribbon, which repeats itself along x-axis. The filled (open) dots stand for the sites on sub-lattice A(B). The three phases for d + id′ pairing gap are defined (see shaded green triangle) as: φ0 = 0, φ1(2) = − (+ )2π/3. superconductor at each end of the wire. Proposals to realize TRITOPs in 2D systems include the spin-triplet px ± ipy superconductors15, the bi-layer Rashba system20, and in exciton condensates21. In this paper, we suggest a novel mechanism for realizing helical Majorana fermions in 2D spin-singlet chiral superconductors with TRS-breaking pairing gap–by directly doping correlated 2D quantum spin Hall insulators (QSHIs or 2D TIs) on honeycomb lattice22,23. A paradigmatic model for QSHIs is the Kane-Mele (KM) model23,24, which shows a non-trivial Z2 topological (or spin Chern) number and supports helical edge states protected by TRS. The half-filled KM model with strong electron correlations is in the Mott-insulating (MI) phase25, while superconductivity appears upon doping. Attractive candidates to realize correlated QSHIs on honeycomb lattice include: graphene with enhanced Kane-Mele SO coupling (∼ 20 meV) by doping with heavy adatoms26, In3Cu2 VO927,28, β–Cu2V2O728,29, and Iridium-based honeycomb compounds X2IrO3(X = Na or Li) with strong SO coupling and electron correlations25,30–32. Via renormalized mean-field theory (RMFT) approach 33,34, we find the spin-singlet TRS breaking d x 2−y 2 + id xy -wave superconductivity to appear at the ground state where the chiral edge states have been shown to occur35. Surprisingly, for sufficiently large SO coupling compared with the superconducting gap, instead of chiral edge states, we find gapless helical MFs to appear at each ribbon edge. This seemingly un-expected feature comes as a result of persistent extension of the quantum spin Hall phase with non-trivial pseudo-spin Chern number upon doping. A novel pseudo-spin Chern to chiral topological quantum phase transition is identified.
Model Hamiltonian. The Hamiltonian of the Kane-Mele t-J (KM-tJ) model is given by23: H = HKM + HJ , HKM = −tgt
∑ ci†α cjα − µ∑ci†α ciα, ij , α
t + i SO 3
νij ci† α σ zcjα ij , α
1 HJ = Jgs ∑ Si ⋅ Sj − ni nj 4 i ,j
+ h. c .
where α = ↑ , ↓ stands for the spin index, 〈 i , j〉 and 〈 〈 i , j〉 〉 refer to the nearest-neighbor (NN) and next-nearest-neighbor (NNN) sites, respectively (see Fig. 1). Here, vij = 1 for i, j ∈ A and vij = − 1 for i, j ∈ Bin the SO coupling; S i refers to the electron spin operator on site i, defined as: S i = 1/2 ∑ α, β =↑, ↓ ci† α σ αβ ciβ , 2 ni = ∑ α ci† α ciα is the electron density operator, and the anti-ferromagnetic spin-exchange couping J ∼ 4t can be U derived via the second-order perturbation from the Kane-Mele Hubbard model in the limit of a strong on-site Coulomb repulsion U ≫ t. Due to breaking of the SU(2) symmetry of the Kane-Mele Hubbard model at half-filling, a small effective ferromagnetic spin-exchange coupling J′ ≪ J term between NNN sites is generated via SO coupling25, which is neglected here (The J′ term favors the magnetic order in XY–plane25 and may induce spin-triplet superconductivity upon doping). We also drop the Rashba SO coupling for simplicity. The HJ term has been known to favor the spin-singlet pairing. To address superconductivity of the model, we apply RMFT based on Gutzwiller projected single-occupancy constraint due to the proximity of the Mott insulating ground states, known to describe the ground state of d–wave cuprate superconductors in qualitative agreement with those via variational Monte Carlo approach33,34.
Scientific Reports | 6:24102 | DOI: 10.1038/srep24102
www.nature.com/scientificreports/ The spin-exchange J term within RMFT reads (see the methods section): H J = H χ + H ∆ + H const , Hχ = H∆ =
∑ χδaci†α ciα+δa + h. c.,
∑∆δa ci†↑ci†+↓δa − ci†↓ci†+↑δa + h.c. , i ,a
2 2 χδ ∆δ a a − 2N µδ , = N s∑ 3 + 3 s g J a 4 gsJ s 4 3 − 4 gs
∑ α J 〈ci† α c α i+δ
(2) 3 − 4 g s J ∑ α , β =↑, ↓ εαβ 〈ciα c β 〉, i+δ a
where a = 1, 2, 3, NS is the total number of sites, χδ = 〉, ∆δ a = a a 2 y and εαβ = iσαβ . Here, g s = 4/(1 + δ ) (see the Methods section). Based on the C6v symmetry of the underlying may take the following forms36,37: (i) extended s–wave: ∆δ = ∆s = ∆0, lattice, the pairing symmetry of ∆δ a = 1,2,3 a δa (ii) d x 2−y 2 + id xy –wave (denoted also as d + id′ ): ∆δ = ∆d +id ′ = ∆0 e i φa−1 with φ0 = 0, φ1(2) = − (+ )2π/3 (see
Fig. 1)38. The Fourier transformed pairing gap Δk for a periodic 2D lattice reads: ∆k = ∑a =1,2,3 ∆δ a e ik⋅δ a. T h e m e a n - f i e l d Ha m i l t o n i a n H k = ψk† k ψk o n a p e r i o d i c l a t t i c e i n t h e b a s i s o f T
ψk = (cA↑ , k, cB↑, k, cA↓ , k, cB↓, k, cA† ↑,−k, cB†,↑−k, cA† ↓,−k, cB†,↓−k ) is given by the 8 × 8 matrix k: hˆ ˆ h + k ∆ k ˆ ˆ , ∆k = k = † , hk = k − ⁎ ∆ ˆ ˆ ˆ hk k −h−k ±γ − µ εk , ∆ = 0 hk± = k ⁎ ∓γ k − µ k ∆−k εk γk =
0 ∆ k −∆ 0 , k ∆k 0
2 t SO − sin(k y ) + 2cos( 3 k x /2) sin(k y /2)], 3
εk = −(t g t + χ)
e ik⋅δ a.
a = 1,2,3
with gt = 2δ/(1 + δ) (see the Methods section). The Hamiltonian Eq. (3) possesses both the Particle-hole (PH) symmetry: C −1Mk C = − M−k, = τ xK (with τx being the Pauli matrix on particle-hole space and K being complex conjugation) as well as sub-lattice symmetry: k → −k for cA,k → cB,k37. The matrix hˆ k , describing the KM model, shows TRS: −1hˆ k = hˆ−k where = iσ yK is the time-reversal operator taking (ck↑, ck↓) to (c−↓k, − c−↑k ) . Howe ver, k bre aks t he TRS for d + id′ sup erconduc ting order parameter : ′ ∆dk +id = cos(π /3)∆d 2 2 (k) + i sin(π /3)∆d (k) w i t h ∆d 2 2 (k) = 2∆0 (e−ik y/ 3 − e ik y/2 cos(k x /2 3 )) , xy
−1 d + id d + id ∆d xy (k) = − 2i∆0 e ik y/2 sin(k x /2 3 ), and T Mk T ≠ M−k . The mean-field free energ y reads: E H 2T F MF = − N ∑k ln cos h 2Tk + Nconst with Ek > 0 being positive eigenvalues and Ns the number of sites. We s s diagonalized the mean-field Hamiltonian Hk on a finite-sized zigzag ribbon with Ns = N/2 zigzag chains and N = 56 is set as the total number of sites along y–axis throughout the paper.
Bulk and edge properties. The mean-field variables are solved self-consistently by minimizing the free
energy both for a periodic lattice and a finite-sized ribbon (see supplementary materials). Compared to the TRS extended s–wave, we find d x 2−y 2 + id xy –wave pairing is the ground state38. Same pairing symmetry has been reported in superconducting phase of the doped graphene in the absence of the spin-orbit coupling35,37,39–41, which was argued to support two co-propagating chiral edge states at low energies with a non-trivial topological winding number NTKNN = ± 242. The superconducting transition temperature Tc is estimated as Tc ∼ gtΔ0. On a finite-sized zigzag ribbon and at a generic doping, the Bogoliubov quasi-particle dispersion shows four doubly-degenerate bulk bands (due to the Sz symmetry of our Hamiltonian) grouped in two pairs (see Fig. 2(a)); it satisfies the particle-hole symmetry with 2π periodicity. At low dopings, the normal state Fermi surfaces enclose the Dirac points K ± = 2π , ± 2π (see Fig. 2(b)); the d + id′ pairing strength is weak near K_38.
Surprisingly, in the regime of a strong SO coupling and weak pairing (∆d+id 3 t SO ), we find the low energy excitations of our model support helical MFs at edges instead of chiral edge states as expected for a chiral d–wave superconductor. On a finite-sized zigzag ribbon, we find two Dirac-dispersed lines intersecting at momenta kxMF ∼ 2π /3, 4π /3 where the Bogoliubov quasi-particle excitation energy vanishes, E (kxMF ) = 0 (see Figs 2(a) and 3(a)). Note that for tSO ≫ Δ0, we find bulk gap closes near kx = 0, π in the pseudo-spin-Chern phase (see Fig. 2). This comes as spin-orbital gap of the pure Kane-Mele ribbon gets smaller near Γ point. Upon doping, the P-H symmetry of the bands is imposed, leading to the overlap between particle and hole bands near kx = 0, π for large tSO/Δ0. We have checked numerically that all the states near kx = 0, π are indeed bulk states. Nevertheless, when t SO is of the same order of magnitude as Δ 0 , we find the bulk gap coloses only at the pseudo-spin-Chern-to-chiral phase transition (see Supplementary materials). Near each of these gapless points, Scientific Reports | 6:24102 | DOI: 10.1038/srep24102
Figure 2. (a) The Bogoliubov dispersion E(kx) (in unit of t) of doped KM-tJ model on a zigzag ribbon with N = 56 for J/t = 0.1, tSO/t = 0.8, and δ = 0.05. (b) The spin-up Fermi surfaces in the normal state of the KaneMele model on 2D periodic lattice for tSO/t = 1 at various dopings. The spin-down Fermi surfaces are obtained via K+ → K−. (c) The 3D density plot for the effective intra-band superconducting gap function ∆−− of the k Kane-Mele model on 2D periodic lattice (see text and Supplementary materials). two pairs of two-fold degenerate states are generated via intersecting the two Dirac lines by a constant energy at MF MF two momentum points k x1(x 2) , denoted as: Ψ1(2), j = 1,2 with the subscript 1(2) being the label of the eigenstate at MF k x1(x 2) and j = 1, 2 the label of two-degenerate eigenstates at a fixed momentum k. These four degenerate states are MF MF MF located at the same edge. However, Ψ1,MF j and Ψ 2,j are counter-propagating, while Ψ j ,1 and Ψ j ,2 are co-propagating (see Fig. 3(b)). These features are clearly different from the co-propagating chiral edge states realized either in the chiral d-wave superconductivity in doped graphene or by proximity of a s–wave superconductor to a quantum anamolous Hall insulators43. Instead, the edge states we find fit well to the helical MFs described by the linearly-dispersed Hamiltonian defined by the Bogoliubov quasi-particle operators γkR (L) τ as: H edge = γkRτ = γkLτ = kxMF , k
k (γ k† Rτ γ kRτ − γ k† Lτ γ kLτ ), k, τ =↑, ↓ ukτ, i ck↑, i + ukτ , i ck↓, i + v kτ , i c−† ↑k , i + vkτ, i c−† k↓ , i, −vkτ, i c−↑k , i + v kτ , i c−↓k , i − uτk , i ck†,↑i + ukτ, i ck†,↓i ,
k x , γ kατ
where k = k − with α = L, R refers to the Bogoliubov quasi-particle destruction operator ≡ defined by the coherence factors ukτ, i , ukτ , i , v kτ , i , vkτ, i , corresponding to the right-moving quasi-particle with “pseudo-spin” τ = ↑ (↓ ), and the summation over repeated site index i = 1, … N is implied; similarly for γ kLτ . The R (L), ↑ (↓) MF ) pair of the degenerate wavefunctions Ψ Rj =(L1(2) (i), formed by the (i) at kxMF 1 (kx 2 ) can be expressed as Ψ coherence factors: Ψ R , ↑(i) = (uk↑, i , u↑k , i , v↑k , i , vk↑, i , ), Ψ L , ↓(i) = ( − vk↓, i , v↓k , i , − u↓k , i , uk↓, i ); similarly for the other dou-
blet Ψ R (L), ↓ (↑) (i). It is clear from Fig. 3(b) that the edge states (Ψ R (L), ↑ (↓), Ψ L (R), ↓ (↑) ) (as well as the Bogoliubov operators (γ kR↑ (L ↓), γ kL ↓ (R↑) )) form pairs (see pink (blue) curve in Fig. 3(b) for |Ψ R , ↑(i) |2 ( Ψ L , ↓(i) 2 )). Scientific Reports | 6:24102 | DOI: 10.1038/srep24102
Figure 3. (a) Bogoliubov excitation spectrum of Fig. 2(a) near zero energy. (b) In the basis of Ψ = [Πi ci↑, Πi ci↓, Πi ci† ↑, Πi ci† ↓ ] with i = 1 … N, the square magnitudes of two pairs of degenerate eigenstate wave-functions associated with the same kxMF is defined as |Ψ (i) |2 ≡ |Ψ Rj =/L1,2 (i) |2 ≡ (|u (i) |2 , |u(i) |2 , |v(i) |2 , |v (i) |2 )Rj /L (see text) for a fixed eigenenergy E = E ± = ± 0.014 t with i running (left to right) from i = 1 (top edge) to i = 56 (bottom edge), corresponding to the helical Majorana fermions. They exhibit an exponential decay from both edges into the bulk. Here, R/L refers to the right/left moving state, and u (i), u(i), v(i), v (i) are the corresponding matrix elements. Physical parameters are the same as in (a). (c) Schematic plot of the helical edge states in (b) for E = E+ where same color in (b,c) refers to the same state. Here, ZGNR refers to the Kane-Mele zigzag nano-ribbon. Furthermore, these Bogoliubov operators with linear dispersion satisfy γ −k( − E ) = γ k† (E ) with k ≡ k − π via PH symmetry (see top and bottom panels of Fig. 3(b)). Hence, they can be regarded as examples of helical MFs at edges15; the MF zero-modes occur at k MF = kxMF − π where γ kατ (E = 0) = γ †ατ (E = 0). An additional symMF −k MF metry is observed due to combined P-H and sublattice symmetries: γ k ( − E ) = γ k† (E ) (see Fig. 3(b)). Our seemingly unexpected results have roots in the competition between TRS SO coupling and TRS breaking chiral d–wave superconductivity. It seems to suggest that the TRS protected Z2 QSH insulating phase of the pure un-doped Kane-Mele model persists up to a finite doping and a finite pairing gap with chiral d-wave narure. To gain more understanding of this surprising result, we try to identify the non-trivial topological invariant corresponding to the helical edge states we found. We first decompose our 8 × 8 Hamiltonian matrix Mk in Eq. 3 ↓ ↑ ↑ ↑ †↓ †↓ in t he ne w b asis cSC into t wo s ep arate d 4 × 4 mat r ices .., HSC , k = (cA , k, cB , k, − cA , −k, cB , −k ) , ↓ ↓ ↓ †↑ †↑ 44 , representing the spin-up and spin-down parts of the M as : cSC = ( c , c , − c , c ) k ,k A ,k B,k A , −k B , −k
Scientific Reports | 6:24102 | DOI: 10.1038/srep24102
γ k − µ k 0 ∆k k⁎ −γ k − µ −∆−k 0 = ⁎ 0 −∆ − γ + µ −k k k ∆⁎ k⁎ 0 γk + k
www.nature.com/scientificreports/ ↓ and similarly for HSC . Due to Sz and sub-lattice symmetries, two pairs of degenerate bands (one pair with positive ↑ ↓ and one with negative eigenvalues) are formed in HSC and HSC . Like the case for the quantum spin-Hall insulator (QSHI), we try to characterize the helical phase of our model in terms of the familar spin Chern number ↑ ( ↓) : C s = (C ↑ − C ↓)/2 where C ↑ (↓) = ∑n Cn↑ (↓). Here, Cn↑ (↓) refers to the Chern number of the nth filled band in HSC 1 ↑ (↓) Cn = 2πi ∫ k∈ BZ F12 (k) where the integral is done in the first Brillouin zone (BZ), the field strength F12(k) and the associated Berry’s connection A(k) are defined as: F12(k) ≡ ∂ 1A2(k) − ∂ 2A1(k) and Aµ = n (k) ∂µ n (k) with ↑ (↓)45 . However, we find C↑ = 0 = C↓ due to the cann (k) being the normalized eigenvector of the nth band in HSC cellation of Cn within each pair of filled degenerate bands. Therefore, the spin Chern number is zero, Cs = 0. ↑ ( ↓) ↑ (↓) ↑ (↓) exhibits an additional pseudo-spin symmetry: τz−1HSC with τz being the z– Nevertheless, HSC τ z = HSC ↑ ( ↓) component of the Pauli matrix defined in 4 × 4 matrix within cSC , k basis, and the pseudo-spin quantum numbers can take ± 1. Therefore, the helical phase realized in our system may still be characterized by a different topological number, similar to the spin Chern number, called the pseudo-spin Chern number C w = (C n − C n)/2 where ↑ ( ↓) , related by (cA↑ , k, cB↑, k ) → ( − cA† ↓, −k, cB†,↓−k ), n and n label the two degenerate bands within each 4 × 4 matrix HSC and carry the opposite pseudo-spin quantum number. In the strong SO coupling regime, tSO ≫ Δ0 and for a sizable range of doping around 1/2-filling, we evaluate Cn, C n numerically and indeed find C n = 1 = −Cn, leading to a ↑ ( ↓) . The total pseudo-spin Chern number by summing over non-trivial pseudo-spin Chern number Cw = 1 for HSC contributions from both spin species is therefore Cwtot = 2 Supplementary materials. Via the bulk-edge correspondence, two pairs of counter-propagating (helical) edge modes are therefore expected, which explains the helical edge states we find numerically via the renormalized mean-field theory. Note that the helical MFs have been known to exist in Z2 TRITOPs and are protected by the time-reversal symmetry (The existence of two pairs of helical edge states via mean-field analysis agrees perfectly with the total spin Chern number being ± 2 via summing over NW for all four filled bands)1,15,46. However, we provide an example of different kind of helical Majorana edge states here which is not protected by TRS, but by the pseudo-spin symmetry. We may call them quasi-helical edge states to be distinguished from the TRS protected helical edge states. These quasi-helical edge states are robust against disorder or spin-nonconserving interactions, similar to the spin-Chern phase in the QSHIs in the absence of TRS47–49. Deep in the pseudo-spin-Chern phase, our system is well approximated by the effective spin-singlet px ± ipy superconductivity near the two Dirac points K±. This can be seen when re-expressing the superconducting pairings in terms of the electron operators ψ±,k which diagonaliz the tight-binding KM Hamiltonian38 Supplementary †↑ †↓ materials. In this basis, the intra-band pairing ∆−− k ψ−, k ψ−, −k dominates at ground state (see Fig. 2(c) and Supplementary materials). Near K± points with q± = K± + (± qx + qy), we find ∆−− q± ∼ ±∆0 (q y ± iqx ), resembling the case of a TRITOPs. In the opposite limit for tSO ≪ Δ0 or sufficiently large doping where the chiral d-wave pairing dominates, however, we recover the chiral superconductivity: NW = 0 and C n = C n = 1, equivalent to the case of doped graphene35,37. A novel pseudo-spin-Chern-to-chiral topological quantum phase transition is identified as Δ0/tSO or μ/tSO is varied (see Supplementary materials)44. The generic phase diagram by tuning μ (in a non-self-consistent way) at a fixed Δ0/tSO is shown in Fig. 4. For Δ0/t ≪ 1, the chiral-to-pseudo-spin-Chern phase transition occurs near ±µc ∼ ± 3 t SO (see Fig. 4(a)). As shown in Fig. 4(b), the bulk band gap closes at the phase boundary μ ∼ − μc at one Dirac point (case (ii)), while it remains finite on either of the two phases (cases (i) and (iii)). For Δ0